Spectroscopic study on the interaction of pristine C60 and serum albumins in solution
© Liu et al.; licensee Springer. 2012
Received: 29 June 2012
Accepted: 24 July 2012
Published: 2 August 2012
The interaction of nanomaterials with biological macromolecules is an important foundation of the design and the biological safety assessments of nanomaterials. This work aims to investigate the interaction between pristine C60 and serum albumins (human serum albumin and bovine serum albumin) in solution. Stable aqueous dispersion of C60 was prepared by simple direct ultrasonic method and characterized by UV–vis spectrophotometry, transmission electronic microscopy and dynamic light scattering techniques, and spectroscopic methods (fluorescence spectroscopy, synchronous fluorescence spectroscopy and circular dichroism spectroscopy) were utilized for the investigation. It was found that the fluorescence of serum albumins could be quenched by C60 nanoparticles in a substantially similar way. Slight changes of the surrounding microenvironment of amino residues were observed, while little effects on the protein secondary structure occurred. The different effects of dispersion methods on the interaction of C60 nanoparticles with serum protein were also compared and discussed.
Studies on the biological effects of nanomaterial are often focused on their cytotoxicity, deposits in target organs and ecological toxicology, while relatively less attention was paid to their interactions with biological macromolecules. Almost all the life processes are inseparable from the participation of biological macromolecules (including proteins and nucleic acids). Following the process of translocation across biological barriers, nanomaterials can be transported into the blood, combine with biological macromolecules in the blood and other tissues, and through the blood transport be deposited in target organs where they exert potential toxic effects[1–3]. Therefore, in-depth understanding of their interactions with biological macromolecules is not only one of the important contents of their potential biomedical applications such as drug delivery, but also related to some basic problems such as the existence of specific roles of the interactions and the biological safety issues of nanomaterials, and thus attracts extensive attention of research communities. However, research on this area is still in its infancy.
Fullerenes are one of the most popular carbon nanomaterials used in industrial manufacturing, synthesis, engineering and medicine. Previous studies already showed that fullerenes (mainly C60 and its derivatives) could exhibit certain cytotoxicity[4, 5], penetrate the blood–brain barrier and be deposited in target organs such as brain, liver, spleen, etc.[6, 7], and cause the DNA damage by oxidative stress. In the research reported about interactions between fullerenes and protein, the majority concentrated in the protein adsorption to the surface of fullerenes and the binding location, while relatively less on the changes of protein conformation and structure[9–11]. Conformation and/or structure changes of a protein induced by being adsorbed to the surface of nanomaterials may result in the changes of its bioactivity, but so far direct evidence of these changes of proteins is sparse. In addition, due to the insoluble nature in water of pristine fullerenes, water-soluble modified fullerene derivatives were often used for the related research. It has been reported that fullerene aqueous dispersions could be obtained by solvent displacement methods or by the addition of surfactant or polymer to water. In the above methods, the organic solvent, surfactant or polymer may affect the accuracy of the experimental results. Among various biological macromolecules, as the most abundant protein in plasma, serum albumin has important physiological functions including the binding and transport of endogenous and exogenous substances. Study on the interaction between fullerenes and serum albumins might help us obtain some information of the transport and removal of fullerenes.
Based on the above, in this work, C60, one of the typical fullerenes, chosen representing nanomaterials, serum albumins (including human serum albumin (HSA) and bovine serum albumin (BSA)) served as subjects, the interaction between C60 and the two serum albumins was investigated by spectroscopic methods. The C60 aqueous dispersion was simply obtained by injecting C60 powder into water, followed by ultrasonic method, and characterized by UV–vis, transmission electron microscopy (TEM) and dynamic light scattering (DLS) techniques. Fluorescence spectroscopy, synchronous fluorescence spectroscopy and circular dichroism (CD) spectroscopy were utilized to investigate the interaction. The binding difference between C60 and two proteins, the location of C60 nanoparticles and the changes of protein conformation and secondary structure were also proposed.
The C60 powder (99.9% pure) was purchased from Puyang Yongxin Fullerene Technology Co. Ltd. (Henan, China) and used as received. HSA and BSA (free fatty acid fraction V) were purchased from Sigma-Aldrich (St. Louis, MO). PBS buffer premixed reagent (pH = 7.4) was obtained from Zhongshan Goldenbridge Biotechnology Co., LTD. (Beijing, China). All solutions were prepared with 18.3 MΩ distilled water (Millipore, USA). Care was taken to minimize exposure of the samples to light during the experiments.
The fluorescence and synchronous fluorescence spectra of proteins were recorded on a FL-4500 Spectrofluorimeter equipped with a 1.0 cm quartz cell. The CD spectra of proteins were recorded on a J-810 Circular Dichroism Spectrometer (Jasco, Japan). UV-1101 spectrophotometer (Shimadzu, Japan), H-7000 transmission electron microscopy (Hitachi, Japan) and BI-200SM/BI-9000 laser light scattering system (Brookhaven, USA) were used to characterize the C60 dispersion. All the measurements were done at room temperature.
Preparation of C60 dispersion
The C60 dispersion was obtained using ultrasonic method. The C60 powder was dissolved in distilled water and sonicated for 48 h. Remove the upper dispersion and abandon the bottom dispersion which contained the undissolved C60 powder. The obtained C60 dispersion was stored in a 4°C refrigerator and dispersed by ultrasound for 30 min before using.
UV–vis absorption spectroscopic measurements
The UV–vis absorption spectra were recorded on a UV-1101 UV–vis recording spectrophotometer (Shimaza, Tokyo, Japan) with a 1.0 cm quartz cell.
Dynamic light scattering measurement
The DLS measurement was performed on a BI-200SM/BI-9000 laser light scattering system (Brookhaven, USA) with a 1.0 cm quartz cell. The measurement was done at room temperature.
Transmission electron microscopic observation
Specimen for TEM observation was prepared by depositing a drop of C60 dispersion on a 150-mesh copper gird and then air-dried in the dark. The TEM image of nC60 nanoparticles was taken from H-7000 transmission electron microscopy (Hitachi).
Fluorescence spectra measurements of proteins
The protein fluorescence measurements were recorded with a FL-4500 spectrofluorimeter in a 1 cm quartz cuvette. The excitation and emission slit width (each 2.5 nm) and scan speed (1200 nm/min) were kept constant for all experiments.
Synchronous fluorescence spectra measurements of proteins
The synchronous fluorescence measurements of proteins were recorded with a FL-4500 spectrofluorimeter in a 1.0 cm quartz cuvette and the excitation and emission slit width were both 2.5 nm with a scan speed of 1200 nm/min. A constant wavelength interval of Δλ = 20 nm or Δλ = 60 nm was set for the measurements.
Circular dichroism spectroscopic measurements of proteins
The CD spectra of proteins were recorded with JASCO-J810 in a 1 mm quartz cuvette with a scan speed of 600 nm/min.
Results and discussion
The UV–vis spectra of C60 dispersions by different preparation methods
As shown in Figure1, there was obvious difference between the absorption spectra of C60 dispersions prepared by the two different methods. For C60 dispersion prepared by direct ultrasonic method (Figure1, line 1), it had absorption in the range of 325–440 nm with a maximum absorption wavelength of 355 nm, while C60 dispersion prepared by solvent replacement (Figure1, line 2) had absorption in the range of 320–440 nm with a maximum absorption wavelength of 344 nm. The shift of the absorption peak of C60 nanoparticles might result from the different morphology and particle size of C60 nanoparticles. The concentration of the prepared C60 dispersion (prepared by direct ultrasonic method) was quantitated by UV–vis spectrophotometry at 344 nm and its concentration was 1.39 × 10-5 mol/L.
Characterization of fullerene dispersion
The TEM image showed C60 nanoparticles were round-like and in the range of 120–260 nm, which agreed well with the average hydrodynamic diameter measured by DLS (The DLS spectrum showed C60 nanoparticles were mainly in the range of 160–500 nm with an average particle size of 283 nm.), and was significantly larger than the values reported previous[13, 16]. The size distribution difference of C60 nanoparticles might be a possible explanation for the difference between the UV–vis absorption spectra in Figure1.
Quenching of protein fluorescence by C60 nanoparticles
The binding of HSA/BSA to C60 nanoparticles
As can be seen from Figure6, the fluorescence intensity of tryptophan residues was 3–4 times that of tyrosine residues, which means the HSA/BSA intrinsic fluorescence is mainly from tryptophan residues. The fluorescence intensity of tryptophan and tyrosine residues could be quenched by the addition of C60 nanoparticles with a dose-effect relationship. For BSA, the maximum emission wavelength of tryptophan residues had a slight blue-shift of about 3–4 nm, while the maximum emission wavelength of tyrosine residues remained basically unchanged, indicating the polarity decrease of the surrounding microenvironment of tryptophan residues. For HSA, consistent with the fluorescence quenching experiment (Figure4), there was no peak wavelength shift of the synchronous fluorescence spectra. In the previous work, the C60 nanoparticles could cause red shift of maximum emission wavelength of tryptophan residues, which was different from this experiment, and we speculated that it might be due to the different size distribution of C60 nanoparticles resulted from the different preparation methods of C60 dispersions.
The secondary structure changes of HSA and BSA
Circular dichroism spectroscopy is an important experimental technique for the study of protein conformation change, which is often used to investigate the secondary and the tertiary structure of proteins. The CD spectra of proteins are generally divided into two wavelength ranges, the far-UV circular dichroism (178–250 nm) and near-UV circular dichroism (250–320 nm). The far-UV region CD spectrum reflects the circular dichroism of peptide bond. The absorption peaks of CD spectra generated from proteins or peptides with different secondary structures were different from each other. By measuring the far-UV CD spectra of proteins or peptides, people could get some information of protein secondary structures, among which 208 nm and 222 nm are the characteristic peaks of α-helix structure[19, 20].
The α-helix and β-sheet structure contents of HSA and BSA
Figure8 showed the CD spectra of HSA and BSA in the absence and presence of C60 nanoparticles. With the addition of C60 dispersion, the absorption of HSA and BSA at 208 nm and 222 nm had slight changes, but no dose–response relationship was observed, which was consistent with the no-significant-difference contents of α-helix and β-sheet structure of HSA and BSA in the absence and presence of C60 nanoparticles (Table1). In the previous work, C60 nanoparticles (prepared by solvent replacement) could cause the α-helix content of HSA increased and the absorption of HSA and BSA at 208 nm and 222 nm weaker with a dose–response relationship. The difference of the two different experimental results may be due to the different sizes of C60 nanoparticles, or residual toluene adsorbed on the surface of C60 nanoparticles in the latter experiment. The mechanism of the difference of protein structure and conformation changes caused by the two prepared C60 nanoparticles need further detailed study.
C60 could be dispersed in water by ultrasonic method as fine clusters. The fluorescence of HSA and BSA could be quenched by C60 nanoparticles by non-specific adsorption. C60 nanoparticles mainly located in the vicinity of tryptophan residues, and caused slight changes of their surrounding microenvironment (only for BSA). During the adsorption process, no obvious changes of the secondary structure of HSA/BSA were observed. Compared with C60 dispersion by solvent exchange method, the C60 dispersion used in this work has little effect on the protein structure, which prompted us to conclude that dispersion method would be important for the bio-safety study of nanomaterials including fullerenes. Direct ultrasonic method can effectivlely avoid the interference of solvents or solubilizer, and thus more accurate for the assessement of the potential toxicity of fullerenes.
The authors acknowledge the considerable support of Innovation Fund for the Post-Doctoral Program of Shandong Province (200902015).
- Zhao XC, Liu RT: Recent progress and perspectives on the toxicity of carbon nanotubes at organism, organ, cell, and biomacromolecule levels. Environ Int 2012, 40: 244–255.View ArticleGoogle Scholar
- Sharifi S, Behzadi S, Laurent S, Forrest ML, Stroeve P, Mahmoudi M: Toxicity of nanomaterials. Chem Soc Rev 2012, 41: 2323–2343. 10.1039/c1cs15188fView ArticleGoogle Scholar
- Buzea C, Blandino IIP, Robbie K: Nanomaterials and nanoparticles: Sources and toxicity. Biointerphases 2007, 2: MR17-MR172. 10.1116/1.2815690View ArticleGoogle Scholar
- Isakovic A, Markovic Z, Nikolic N, Todorovic-Markovic B, Vranjes-Djuric S, Harhaji L, Raicevic N, Romcevic N, Vasiljevic-Radovic D, Dramicanin M, Trajkovic V: Inactivation of nanocrystalline C60 cytotoxicity by gamma-irradiation. Biomaterials 2006, 27: 5049–5058. 10.1016/j.biomaterials.2006.05.047View ArticleGoogle Scholar
- Zhao BZ, He YY, Bilski PJ, Chignell CF: Pristine (C60) and hydroxylated [C60 (OH) 24] fullerene phototoxicity towards HaCaT keratinocytes: Type I vs Type II Mechanisms. Chem Res Toxicol 2008, 21: 1056–1063. 10.1021/tx800056wView ArticleGoogle Scholar
- Moussa F, Trivin F, Céolin R, Hadchouel M, Sizaret PY, Greugny V, Fabre C, Rassat A, Szwarc H: Early effects of C60 admininstration in swiss mice: a preliminary account for in vivo C60 toxicity. Fullerene Sci Technol 1996, 4: 21–29. 10.1080/10641229608001534View ArticleGoogle Scholar
- Oberdörster E: Manufactured nanomaterials (Fullerenes, C60) induce oxidative stress in the brain of juvenile largemouth bass. Environ Health Perspect 2004, 112: 1058–1062. 10.1289/ehp.7021View ArticleGoogle Scholar
- Folkmann JK, Risom L, Jacobsen NR, Wallin H, Loft S, Møller P: Oxidatively Damaged DNA in Rats Exposed by Oral Gavage to C60 Fullerenes and Single-Walled Carbon Nanotubes. Environ Health Perspect 2009, 117: 703–708.View ArticleGoogle Scholar
- Benyamini H, Shulman-Peleg A, Wolfson HJ, Belgorodsky B, Fadeev L, Jozin M: Interaction of C60-Fullerene and carboxyfullerene with proteins: Docking and binding site alignment. Bioconjugate Chem 2006, 17: 378–386. 10.1021/bc050299gView ArticleGoogle Scholar
- Deguchi S, Yamazaki T, Mukai S, Usami R, Horikoshi K: Stabilization of C60 nanoparticles by protein adsorption and its implications for toxicity studies. Chem Res Chem Res Toxicol 2007, 20: 854–858. 10.1021/tx6003198View ArticleGoogle Scholar
- Rozhkov SP, Goryunov AS, Sukhanova GA, Borisova AG, Rozhkova NN, Andrievsky GV: Protein interaction with hydrated C60 fullerene in aqueous solutions. Biochem Biophys Res Commun 2003, 303: 562–566. 10.1016/S0006-291X(03)00392-9View ArticleGoogle Scholar
- Belgorodsky B, Fadeev L, Ittah V, Benyamini H, Zelner S, Huppert D, Kotlyar AB, Gozin M: Formation and characterization of stable human serum albumin-tris-malonic acid [C60] fullerene complex. Bioconjugate Chem 2005, 16: 1058–1062. 10.1021/bc050103cView ArticleGoogle Scholar
- Song MY, Liu SF, Yin JF, Wang HL: Interaction of Human Serum Album and C60 Aggregates in Solution. Int J Mol Sci 2011, 12: 4964–4974. 10.3390/ijms12084964View ArticleGoogle Scholar
- Torresa VM, Posac M, Srdjenovicc B, Simplícioa AL: Solubilization of fullerene C60 in micellar solutions of different solubilizers. Colloid Surfac B 2011, 82: 46–53. 10.1016/j.colsurfb.2010.08.012View ArticleGoogle Scholar
- Popov VA, Tyunin MA, Zaitseva OB, Karaev RH, Sirotinkin NV, Dumpis MA, Piotrovsky LB: C60/PVP complex — No Toxicity after Introperitoneal Injection to Rats. Fuller Nanotub Car N 2008, 16(5–6):693–697.View ArticleGoogle Scholar
- Deguchi S, Alargova RG, Tsujii K: Stable Dispersions of Fullerenes, C60 and C70, in Water. Preparation and Characterization. Langmuir 2001, 17: 6013–6017. 10.1021/la010651oView ArticleGoogle Scholar
- Benesch J, Hungerford G, Suhling K, Tregidgo C, Mano JF, Reis RL: Fluorescence probe techniques to monitor protein adsorption-induced conformation changes on biodegradable polymers. J Colloid Interf Sci 2007, 312: 193–200. 10.1016/j.jcis.2007.03.016View ArticleGoogle Scholar
- Goodpaster JV, Mcguffin VL: Rapid and Accurate Determination of Stern-Volmer Quenching Constants. Appl Spectrosc 1999, 53: 1000–1008. 10.1366/0003702991947676View ArticleGoogle Scholar
- Brahms S, Brahm J: Determination of protein secondary structure in solution by vacuum ultraviolet circular dichroism. J Mol Biol 1980, 138: 149–178. 10.1016/0022-2836(80)90282-XView ArticleGoogle Scholar
- Messina P, Prieto G, Dodero V, Cabrerizo-Vilchez MA, Aldonado-Valderrama J, Ruso JM, Sarmiento F: Surface characterization of human serum albumin and sodium perfluorooctanoate mixed solutions by pendant drop tensiometry and circular dichroism. Biopolymers 2006, 82: 261–271. 10.1002/bip.20494View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.